Designation: A179/A179M − 90a (Reapproved 2012)
Used in USNRC-RDT Standards
Standard Speciﬁcation for
Seamless Cold-Drawn Low-Carbon Steel Heat-Exchanger and Condenser Tubes 1 This standard is issued under the ﬁxed designation A179/A179M; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revis revision. ion. A number in parentheses parentheses indicates the year of last reapproval. reapproval. A superscript epsilon (´) indicates an editorial change since the last revision or reapproval.
1. Sco Scope pe 1.1 This spec speciﬁcati iﬁcation on2 covers minimum-wall-th minimum-wall-thickness, ickness, seamless cold-drawn low-carbon steel tubes for tubular heat exchangers, condensers, and similar heat transfer apparatus. 1.2 This speciﬁcation speciﬁcation covers tubes 1 ⁄ 8 to 3 in. [3.2 to 76.2 mm], inclusive, in outside diameter. NOTE 1—Tubing smaller in outside diameter and having a thinner wall than ind indica icated ted in thi thiss spe speciﬁ ciﬁcat cation ion is ava availa ilable ble.. Mec Mechan hanica icall pro proper perty ty requir req uireme ements nts do not app apply ly to tub tubing ing sma smalle llerr tha than n 1 ⁄ 8 in. [3.2 mm] in outside diameter or with a wall thickness under 0.015 in. [0.4 mm].
1.3 The values stated in either inch-poun inch-pound d units or SI units are to be regarded separately as standard. Within the text, the SI un units its ar aree sh show own n in br brac acke kets ts.. Th Thee va valu lues es sta state ted d in eac each h system are not exact equivalents; therefore, each system must be used independently of the other. Combining values from the two systems may result in nonconformance with the speciﬁcatio cat ion. n. Th Thee in inch ch-p -pou ound nd un units its sh shal alll ap appl ply y un unles lesss th thee “M “M”” designation of this speciﬁcation is speciﬁed in the order. 2. Referenc Referenced ed Documents Documents 2.1 ASTM Standards:3 A450/A450M Speciﬁc Speciﬁcation ation for Gener General al Requir Requirements ements for Carbon and Low Alloy Steel Tubes 3. Orde Ordering ring Information Information 3.1 Or 3.1 Orde ders rs fo forr mat mater erial ial un unde derr th this is sp spec eciﬁ iﬁcat catio ion n sh shou ould ld include incl ude the fol follow lowing ing,, as req requir uired, ed, to des describ cribee the des desired ired material adequately: 3.1.1 Quanti Quantity ty (feet, metres, or numbe numberr of length lengths), s), 3.1.2 Name of material (seamless (seamless tubes), 3.1.3 Manufacture (cold-drawn), (cold-drawn), 1
This speciﬁcation is under the jurisdiction of ASTM Committee A01 A01 on on Steel, Stainless Steel and Related Alloys and is the direct responsibility of Subcommittee A01.09 on A01.09 on Carbon Steel Tubular Products. Current edition approved March 1, 2012. Published November 2012. Originally approved in 1935. Last previous edition approved in 2005 as A179/A179M – 90a (2005). DOI: 10.1520/A0179_A0179M-90AR12. 2 For ASME Boile Boilerr and Pres Pressure sure Vessel Vessel Code appli application cationss see related Spec Speciﬁiﬁcation SA-179 in Section II of that Code. 3 For referenced ASTM standards, visit the ASTM website, www.astm.org, or contact ASTM Customer Service at [email protected]
For Annual Book of ASTM Standards volume information, refer to the standard’s Document Summary page on the ASTM website.
3.1.4 Size (outside (outside diameter and minimum wall thickness), thickness), 3.1.5 Length (speciﬁc (speciﬁc or random), random), 3.1.6 Option Optional al requir requirements ements (product analys analysis, is, Sectio Section n 9, ﬂange test, 11.3 test, 11.3), ), 3.1.7 Test report required (Certiﬁcation (Certiﬁcation Section of Speciﬁ Speciﬁ-cation A450/A450M cation A450/A450M), ), 3.1.8 Speciﬁ Speciﬁcation cation number, number, and 3.1.9 Specia Speciall requi requirement rements. s. 4. General Requirements Requirements 4.1 Mat Materia eriall fur furnis nished hed und under er thi thiss spe speciﬁ ciﬁcati cation on sha shall ll con con-form to the applicable requirements of the current edition of Speciﬁcation A450/A450M Speciﬁcation A450/A450M,, unless otherwise provided herein. 5. Manu Manufactu facture re 5.1 Tub Tubes es shall be made by the seamless process process and shall be cold drawn. 6. Heat Treatmen Treatmentt 6.1 Tub Tubes es shall be heat treated after after the ﬁnal cold draw pass pass at a temperature of 1200°F [650°C] or higher. 7. Surfa Surface ce Condition Condition 7.1 Finish Finished ed tubes shall be free of scale. A slight slight amount amount of oxidation will not be considered as scale. 8. Chem Chemical ical Compositio Composition n 8.1 The steel shall conform conform to the follow following ing requirements requirements as to chemic chemical al compo composition: sition: Carbon, % M an g an es e , % Phosphorus, max, % Sulfur, max, %
0 .0 6 – 0 .1 8 0 .2 7 – 0 .6 3 0 .0 3 5 0 .0 3 5
8.2 Suppl Supplying ying an alloy grade that speciﬁcally requires requires the addition of any element other than those listed in 8.1 is not permitted. 9. Pro Product duct Analysi Analysiss 9.1 When requested requested on the purch purchase ase order, order, a prod product uct analysis shall be made by the supplier from 1 tube per 250 pieces or when tubes are identiﬁed by heat, one tube per heat shall be analyz ana lyzed. ed. The che chemica micall com compos positio ition n thu thuss det determ ermine ined d sha shall ll conform to the requirements speciﬁed.
Copyright © ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959. United States
Copyright by ASTM Int'l (all rights reserved); reserved); Tue Dec 4 01:09:37 EST 2012 1 Downloaded/printed by (Book Supply Bureau) pursuant to License Agreement. No further reproductions authorized.
A179/A179M − 90a (2012) 9.2 If the original test for product analysis fails, retests of two additional billets or tubes shall be made. Both retests, for the elements in question, shall meet the requirements of the speciﬁcation; otherwise all remaining material in the heat or lot (Note 2) shall be rejected or, at the option of the producer, each billet or tube may be individually tested for acceptance. Billets or tubes which do not meet the requirements of the speciﬁcation shall be rejected. NOTE 2—A lot consists of 250 tubes.
10. Hardness Requirements 10.1 The tubes shall have a hardness number not exceeding 72 HRB. 11. Mechanical Tests Required 11.1 Flattening Test— One ﬂattening test shall be made on specimens from each of two tubes from each lot (Note 2) or fraction thereof. 11.2 Flaring Test— One ﬂaring test shall be made on specimens from each of two tubes from each lot (Note 2) or fraction thereof. 11.3 Flange Test— When speciﬁed as a substitute for the ﬂaring test, for tubes having a wall thickness (actual mean wall) less than 10 % of the outside diameter, one test shall be made on specimens from each of two tubes from each lot (Note
2) or fraction thereof. For tubes other than speciﬁed above, the ﬂange test shall not be required. 11.4 Hardness Test— Rockwell hardness tests shall be made on specimens from two tubes from each lot. The term lot applies to all tubes, prior to cutting, of the same nominal diameter and wall thickness which are produced from the same heat of steel. When ﬁnal heat treatment is in a batch-type furnace, a lot shall include only those tubes of the same size and the same heat which are heat treated in the same furnace charge. When the ﬁnal heat treatment is in a continuous furnace, a lot shall include all tubes of the same size and heat, heat treated in the same furnace at the same temperature, time at heat, and furnace speed. 11.5 Hydrostatic Test— Each tube shall be subjected to the hydrostatic test, or, instead of this test, a nondestructive electric test may be used when speciﬁed by the purchaser. 12. Product Marking 12.1 In addition to the marking prescribed in Speciﬁcation A450/A450M, the marking shall include the name and order number of the purchaser. 13. Keywords 13.1 cold drawn tube; condenser tubes; heat exchanger tubes; low carbon steel; seamless tube
EXPLANATORY NOTES NOTE 1—For purposes of design, the following tensile properties may be assumed: Tensile strength, min, ksi [MPa] Yield strength, min, ksi [MPa] Elongation in 2 in. or 50 mm, min, %
47  26  35
ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or [email protected]
(e-mail); or through the ASTM website (www.astm.org). Permission rights to photocopy the standard may also be secured from the ASTM website (www.astm.org/ COPYRIGHT/).
Copyright by ASTM Int'l (all rights reserved); Tue Dec 4 01:09:37 EST 2012 2 Downloaded/printed by (Book Supply Bureau) pursuant to License Agreement. No further reproductions authorized.